DOI 10.1007/s10948-012-1743-6

O R I G I N A L PA P E R

**Muon-Spin Rotation and Magnetization Studies of Chemical**

**and Hydrostatic Pressure Effects in EuFe**

**2**

**(As**

**1**

**−x**

**−x**

**P**

**x**

**x**

**)**

**2**

**Z. Guguchia· A. Shengelaya · A. Maisuradze ·**

**L. Howald· Z. Bukowski · M. Chikovani · H. Luetkens ·**
**S. Katrych· J. Karpinski · H. Keller**

Received: 24 July 2012 / Accepted: 30 July 2012 / Published online: 25 August 2012 © Springer Science+Business Media, LLC 2012

**Abstract The magnetic phase diagram of EuFe**2(As1*−x*P*x*)2
was investigated by means of magnetization and muon-spin
*rotation (μSR) studies as a function of chemical (isovalent*
substitution of As by P) and hydrostatic pressure. The
mag-netic phase diagrams of the magmag-netic ordering of the Eu and
Fe spins with respect to P content and hydrostatic pressure
are determined and discussed. The present investigations
re-veal that the magnetic coupling between the Eu and the Fe
sublattices strongly depends on chemical and hydrostatic

Z. Guguchia (

)· A. Maisuradze · L. Howald · H. Keller Physik-Institut der Universität Zürich, Winterthurerstrasse 190, 8057 Zürich, Switzerlande-mail:zurabgug@physik.uzh.ch

A. Shengelaya· M. Chikovani

Department of Physics, Tbilisi State University, Chavchavadze 3, 0128 Tbilisi, Georgia

*Present address:*

M. Chikovani

Laboratory for Developments and Methods, Paul Scherrer Institute, 5232 Villigen PSI, Switzerland

A. Maisuradze· H. Luetkens

Laboratory for Muon Spin Spectroscopy, Paul Scherrer Institute, 5232 Villigen PSI, Switzerland

*Present address:*

Z. Bukowski

Institute of Low Temperature and Structure Research, Polish Academy of Sciences, 50-422 Wroclaw, Poland

Z. Bukowski· S. Katrych · J. Karpinski

Laboratory for Solid State Physics, ETH Zürich, 8093 Zürich, Switzerland

*Present address:*

S. Katrych· J. Karpinski

Institut de Physique de la Matiére Condensée (ICMP), Ecole Polytechnique Fédérale de Lausanne (EPFL), 1015 Lausanne, Switzerland

pressure. It is found that chemical and hydrostatic pressures have a similar effect on the Eu and Fe magnetic order.

**Keywords High temperature Fe-based superconductor**·
Localized and band magnetism· Hydrostatic pressure ·
Chemical pressure

**1 Introduction**

The discovery of superconductivity in the iron-based
pnic-tides [1] provided a new class of compounds to the high
temperature superconductor (HTS) family. Ternary iron
*ar-senide AFe*2As2*(A*= Sr, Ca, Ba, Eu) [2] is one of the
par-ent compounds with ThCr2Si2-type structure. Similarly as
*LnFeAsO (Ln*= La–Gd) [3*], AFe*2As2undergoes a
struc-tural phase transition from a tetragonal to an
orthorom-bic phase, accompanied or followed by a spin-density-wave
(SDW) transition of the itinerant Fe moments. The
super-conducting (SC) state can be achieved either under pressure
(chemical and hydrostatic) [4–6] or by appropriate charge
carrier doping of the parent compounds [7–9], both
accom-panied by a suppression of the SDW state.

Here, we focus on EuFe2As2which is a particularly
*inter-esting member of the ternary system AFe*2As2*, since the A*
site is occupied by a rare earth Eu2+*S*-state (orbital moment
*L= 0) ion with a 4f*7electronic configuration. Eu2+has a
*total electron spin S= 7/2, corresponding to a theoretical*
*effective magnetic moment of μ*eff*= 7.94 μB*. In addition to
*the SDW ordering of the Fe moments at T*SDW 190 K, an
antiferromagnetic (AFM) order of the Eu2+*spins at T*AFM
19 K was reported by Mössbauer spectroscopy [10] and later
confirmed by neutron diffraction [11]. Various reports on
EuFe2*−x*Co*x*As2*(x*= 0 and 0.1) suggest a strong coupling
between the magnetism of the Eu2+ions and the conduction
electrons, which may affect or even destroy

superconductiv-ity [12,13]. For example, in contrast to the other ‘122’
sys-tems, where the substitution of Fe by Co leads to
supercon-ductivity [14,15], the compounds containing Eu2+ exhibit
the onset of a superconducting transition, but seem to be
hindered to reach zero resistivity at ambient pressure [16].
Although Ni doping in BaFe2As2leads to superconductivity
up to 21 K [17], ferromagnetism rather than
superconductiv-ity was found in EuFe2As2by Ni doping [18]. On the other
hand, in single crystals of P substituted EuFe2(As1*−x*P*x*)2
bulk superconductivity with superconducting transition
*tem-perature T*c 28 K was observed by resistivity,
magnetiza-tion, and specific heat measurements [19]. Isovalent P
sub-stitution on the As site in EuFe2As2 without introducing
holes or electrons simulates a condition generally referred to
as “chemical pressure”. Superconductivity coexisting with
AFM Eu2+order was only found in a very narrow range of
*P content x (0.16≤ x ≤ 0.22), where the SDW transition is*
suppressed. Superconductivity with a zero resistivity state
was also observed for EuFe2As2 under applied pressure
[6,20]. Similar to the case of P substitution,
superconduc-tivity covers only a narrow pressure range of 2.5–3.0 GPa.

In this paper, we report detailed magnetization and muon
*spin rotation (μSR) measurements in EuFe*2As2*−x*P*x* as
*a function of the P content x. One P substituted sample*
EuFe2(As*0.88*P*0.12*)2 was also studied under applied
*pres-sure p. The μSR technique is a powerful tool to study*
the magnetic and superconducting properties of materials
*microscopically. It provides reliable measurements of T*c,
*TSDW*, the magnetic ordering temperature of Eu2+ spins
*T*Eu *and the ordered moment size as a function of both x*
*and p. Consequently, the phase diagrams with respect x and*
*p*are determined from these measurements. We compare the
present results with previous high pressure studies on the
parent compound EuFe2As2 and discuss the combined
*re-sults in terms of the relation of x and p. The paper is *
or-ganized as follows: Experimental details are described in
Sect. 2. The results of the magnetic susceptibility and the
*μ*SR experiments at ambient and applied pressure are
pre-sented and discussed in Sects.3.1and3.2, respectively. In
Sect.4, the phase diagrams are presented. The conclusions
follow in Sect.5.

**2 Experimental Details**

In the present work, the system EuFe2(As1*−x*P*x*)2 with
*x* = 0, 0.12, 0.2, and 1 is investigated. Note that the
*sam-ple with x*= 0 is single crystalline, and all the P
substi-tuted compounds are pollycrystalline. The concentrations
*x= 0.12 and 0.2 were studied due to their proximity to the*
SC phase reported in [19]. A single crystal of EuFe2As2was
grown out of Sn flux [21]. Polycrystalline samples were
syn-thesized by solid-state reaction between EuAs, Fe2As, and
Fe2P. EuAs was presynthesized by heating europium grains
and phosphorus powders very slowly to 1173 K followed

by a tempering at this temperature for 36 h. Fe2As was pre-pared by heating Fe and As powders at 973 K for 10 h and at 1173 K for 15 h. Fe2P was presynthesized by reacting iron and phosphorus powders at 973 K for 24 h from sto-ichiometric amounts of the elements. All the starting ma-terials had a purity better than 99.9 %. Powders of EuAs, Fe2As, and Fe2P were weighted according to the stoichio-metric ratio, thoroughly ground and pressed into pellets in an argon-filled glove box. The pellets were then sealed in an evacuated quartz tube, sintered at 1273 K for 36 h, and then cooled slowly to room temperature.

Powder X-ray diffraction (XRD) studies of the
EuFe2(As1* _{−x}*P

*x*)2 samples were carried out at room tem-perature with a STOE diffractometer (CuK

*α1*radiation,

*λ= 1.5406 Å) equipped with a mini-phase-sensitive*de-tector and a Ge monochromator. The structural refinements were done using the program FULLPROF [22]. The zero-field-cooled and zero-field-cooled (ZFC and FC) magnetization measurements of the EuFe2(As1

*−x*P

*x*)2 samples were

*per-formed with a commercial SQUID magnetometer (Quantum*

*Design MPMS-XL). The samples with x= 0.2 and 1 were*

*studied only at ambient pressure. For x= 0.12, the*investi-gations were also carried out under applied pressures up to

*p= 5.9 GPa by using a diamond anvil cell (DAC) filled with*Daphne oil which served as a pressure-transmitting medium. The pressure at low temperatures was determined by the pressure dependence of the SC transition temperature of Pb.

*Zero-field (ZF) μSR experiments were performed at*

*the μE1 and π M3 beamlines of the Paul Scherrer*Insti-tute (Villigen, Switzerland). The general purpose instru-ment (GPS) was used to study the system EuFe2(As1

*−x*P

*x*)2

*(x*= 0, 0.12, 0.2, and 1) at ambient pressure. The sam-ples were mounted inside of a gas-flow 4He cryostat on a sample holder with a standard veto setup providing a

*low-background μSR signal. In addition, the sample with*

*x= 0.12 was studied under pressure using the GPD*instru-ment. Pressures up to 2.0 GPa were generated in a double wall piston-cylinder type of cell made of MP35N [23]

*ma-terial especially designed to perform μSR experiments*un-der pressure. As a pressure transmitting medium Daphne oil was used. The pressure was measured by tracking the SC transition of a very small indium plate by AC susceptibility.

*The μSR time spectra were analyzed using the free software*package MUSRFIT [24].

**3 Results and Discussion**

3.1 Crystal Structure and Magnetic Properties
of EuFe2(As1* _{−x}*P

*x*)2

*3.1.1 X-Ray Powder Diffraction*

The crystal structure for all EuFe2(As1*−x*P*x*)2 samples at
room temperature was refined with the tetragonal ThCr2Si2

**Fig. 1 X-ray powder diffraction pattern at room temperature for the**

sample EuFe2(As*0.88*P*0.12*)2*. The solid line represents a Ritveld *

*refine-ment profile. The residuals are plotted at the bottom of the figure. In the*

*inset, refined lattice parameters are plotted as a function of P content x*

structure. An example of the refinement profile for
EuFe2(As*0.88*P*0.12*)2 is shown in Fig. 1. No obvious
sec-ondary phase can be detected. The weighted pattern
*fac-tor and goodness of fit are Rwp∼ 11.2 % and S ∼ 1.6,*
respectively, indicating a fairly good refinement. In
ad-dition, the refined occupancies are close to the nominal
values. The lattice constants for the tetragonal unit cell
*based upon the Rietveld refinements are a= 3.9095(2) Å*
*and c* *= 11.979(1) Å for x = 0.12, a = 3.9006(2) Å*
*and c= 11.9312(1) Å for x = 0.2, a = 3.8152(2) Å and*
*c= 11.2401(1) Å for x = 1. The values for x = 1 are in*
*agreement with the literature values [a= 3.8178(1) Å and*
*c= 11.2372(3) Å] [*25*]. The lattice constants a and c as*
*a function of x are plotted in the inset of Fig.* 1. A
*de-crease of both a and c with increasing x is observed. The*
*decrease of the lattice constant c as a result of P *
substi-tution implies an increase of the coupling between the Eu
and the Fe2(As1*−x*P*x*)2layers. This might also be important
for the evolution of the magnetic order in the Eu-sublattice,
since the Ruderman–Kittel–Kasuya–Yosida (RKKY)
cou-pling strongly depends on the distance between the magnetic
ions [13,18,25].

*3.1.2 Magnetization Measurements*

The temperature dependence of the zero-field-cooled (ZFC)
*and field-cooled (FC) magnetic susceptibility χ= M/H for*
EuFe2(As1*−x*P*x*)2*(x= 0.12, 0.2, and 1) in a magnetic field*
*of μ*0H= 2 mT is shown in Fig. 2*. The results for x*= 0
were already discussed in detail in our previous work [21],
and hence, are not shown here. The magnetic susceptibility
at high temperatures (i.e., far above the magnetic ordering
temperature of the Eu2+_{moments T}

Eu) is well described by

**Fig. 2 Temperature dependence of the ZFC and FC magnetic **

suscep-tibility for the samples EuFe2(As1*−x*P*x*)2*(x= 0.12, 0.2, 1) measured*

*in a magnetic field of μ*0*H= 2 mT. The inset illustrates the *

*tempera-ture dependence of the difference of both susceptibilities (χ*FC*−χ*ZFC).

*The arrows mark the magnetic ordering temperatures T*Euof the Eu2+

moments

the Curie–Weiss law:
*χ (T )*= *C*

*T* *− θ*CW

*.* (1)

*Here, C denotes the Curie constant and θ*CW the
paramag-netic Curie–Weiss temperature. An analysis of the data in
Fig.2with Eq. (1*) yields: θ*CW*= 16.74(8) K, μ*eff* 8.1 μB*
*for x= 0.12, θ*CW*= 18.14(7) K, μ*eff* 8.2 μBfor x= 0.2,*
*and θ*CW*= 29.35(9) K, μ*eff* 8.3 μB* *for x*= 1. The
*ob-tained values of μ*eff are close to the theoretical value of a
free Eu2+*ion (μ*Eu2+*= 7.94 μB*).

As shown in Fig.2, for all the P substituted samples an
*obvious deviation between χ*ZFC*and χ*FCis seen at low
*tem-peratures. This is not the case for x*= 0 [18,21], for which
AFM order of Eu2+ with the moments pointing along the
*a* axis was reported. This result is consistent with previous
magnetizaton studies [26], suggesting that the ground state
of the coupled Eu2+spins is a canted AFM state (C-AFM
state) (i.e., AFM with the net ferromagnetic (FM)
*compo-nent along the c-axis) in EuFe*2(As1*−x*P*x*)2*(x= 0.12, 0.2)*
and a FM state in EuFe2P2. Recently, neutron diffraction
measurements were also performed on EuFe2P2and an
al-most axial FM structure of the Eu2+spins was established
[27]. The C-AFM and FM structure of the Eu-sublattice in
EuFe2(As1*−x*P*x*)2*(x= 0.12, 0.2, 1) sharply contrasts with*
the planar antiferromagnetism seen in the parent compound
EuFe2As2, suggesting a delicate interplay between the Eu
*4f and the Fe 3d electrons. It was concluded from different*
experiments [12,13] that there is a strong coupling between
the localized Eu2+_{spins and the conduction electrons of the}
two-dimensional (2D) Fe2As2layers in EuFe2As2. This
re-vealed that the magnetic exchange interaction between the

**Fig. 3 ZF μSR spectra for**

EuFe2(As1*−x*P*x*)2*(x*= 0, 0.12,

0.2, 1) recorded for three
*different temperatures: T < T*Eu

*(circles), T*Eu*< T < T*SDW

*(diamonds), and T > T*SDW

*(spheres). The solid lines*
represent fits to the data by
means of Eq. (2)

*localized Eu 4f moments is mediated by the itinerant Fe*
*3d electrons. However, the interaction of the Eu moments*
with the magnetic moments of the Fe sublattice (band
mag-netism) cannot be neglected. Only a combination of both
interactions can further elucidate the C-AFM ground state
observed in EuFe2(As1*−x*P*x*)2*(x= 0.12 and 0.2). Note that*
a C-AFM ground state was also found in the related
com-pound EuFe*1.8*Co*0.2*As2[21].

*The magnetic ordering temperature T*Euof the Eu2+
mo-ments was determined by the temperature at which the
*dif-ference between χ*ZFC *and χ*FC sets in (see the inset of
Fig. 2*). It was found to be T*Eu* 16.5, 18, and 29 K for*
*x= 0.12, x = 0.2, and x = 1, respectively. The value of T*Eu
*for x= 0.12 is slightly reduced compared to T*Eu 19 K for
*the parent compound x*= 0. However, on further increasing
*the P concentration T*Euincreases and reaches a maximum
*for x= 1. The value of T*Eu*for x*= 1 is in agreement with
those reported in literature [19,25,27].

*3.1.3 Zero-Field μSR Measurements*

*In a μSR experiment, nearly 100 % spin-polarized muons*
*μ*+are implanted into the sample one at a time. The
*pos-itively charged μ*+ thermalize at interstitial lattice sites,
where they act as magnetic microprobes. In a magnetic
material, the muon spin precesses in the local magnetic
*field Bμ* at the muon site with the Larmor frequency
*νμ* *= γμ/(2π )Bμ* *(muon gyromagnetic ratio γμ/(2π )*=
*135.5 MHz T*−1*). ZF μSR is a very powerful tool to *
in-vestigate microscopic magnetic properties of solids without
applying an external magnetic field.

*ZF μSR time spectra for the single crystal of EuFe*2As2
and for the polycrystalline samples EuFe2(As1*−x*P*x*)2 are
shown in Fig.3, recorded for three different temperatures:
*T < T*Eu*, T*Eu*< T < T*SDW*, and T > T*SDW. For EuFe2As2,
*the ZF μSR measurements were performed with the initial*
muon spin polarization tilted by approximately 45◦ away
*from the crystallographic c-axis. At high temperatures (see*
Fig.3), no muon spin precession and only a very weak
*polarization of the μSR signal is observed. This weak *
de-polarization and its Gaussian functional form are typical
for a paramagnetic material and reflect the occurrence of
a small Gaussian–Kubo–Toyabe depolarization, originating
from the interaction of the muon spin with randomly
ori-ented nuclear magnetic moments. At temperatures below
*TEu*a well-defined spontaneous muon spin precession is
ob-served in all compounds, indicating long-range magnetic
or-der of the Eu2+ moments in the investigated compounds.
*For x= 0 and 0.12 above T*Eu* 20.5 and 16.5 K, *
respec-tively, muon spin precession with a lower frequency is
ob-served which is caused by the long-range SDW order of the
*Fe moments. However, for x= 0.2, instead of the *
*oscilla-tory behavior seen in the SDW state for x*= 0 and 0.12,
a fast decaying signal is observed (see Fig.3(c)). The
*rea-son for this strongly decaying μSR signal will be discussed*
*below. For x*= 1, only the magnetic ordering of the Eu
*mo-ments is seen in the μSR spectra (Fig.*3(d)). Note that for
*x= 0, 0.12 and 0.2 only one μSR frequency is visible. *
*How-ever, for x*= 1 two distinct precession frequencies occur in
*the μSR spectra, corresponding to the local magnetic fields*
*B _{μ,Eu}*1

*1.08 T (70 % of the signal) and B*2

_{μ,Eu}*1.37 T*

**Fig. 4 The temperature dependence of the internal magnetic field B**i*μ*

for the samples EuFe2(As1*−x*P*x*)2*(x= 0, 0.12, 0.2, and 1). The solid*

*lines represent fits to the data by means of Eq. (*3*). The arrows mark*
*the transition temperatures for the SDW (T*SDW) and the Eu magnetic

*order (T*Eu)

(30 % of the signal). This indicates that two magnetically inequivalent muon stopping sites are present in EuFe2P2.

*The ZF μSR data were analyzed using the following*
functional form:
*A(t )*=
2
*i*=1
*Ai*_{0}*αie−λ*
*i*
*Tt*_{cos}_{γ}_{μ}_{B}i*μt+ ϕ*
*+ βie−λ*
*i*
*Lt*_{.}_{(2)}

*αi* *and βi= 1 − αi* *(i= 1 for x = 0, 0.12, 0.2, and i = 1, 2*
*for x*= 1) are the fractions of the oscillating and
*nonoscil-lating μSR signal. For the single crystal (x*= 0) one finds
*α*1*= 0.73(2) and β*1*= 0.27(3). However, for the *
*polycrys-talline samples αi= 2/3 and βi* *= 1/3. The 2/3 oscillating*
*and the 1/3 nonoscillating μSR signal fractions originate*
from the spatial averaging in powder samples where only
*2/3 of the magnetic field components are perpendicular to*
*the muon spin and cause muon spin precession. A*0denotes
*the initial asymmetry, and ϕ is the initial phase of the *
*muon-spin ensemble. Bi*

*μ*represents the internal magnetic field at
*the muon site, and the depolarization rates λi _{T}*

*and λi*char-acterize the damping of the oscillating and nonoscillating

_{L}*part of the μSR signal, respectively. The transversal*

*relax-ation rate λi*is a measure of the width of the static mag-netic field distribution at the muon site, and also reflects dynamical effects (spin fluctuations). The longitudinal

_{T}*re-laxation rate λi*is determined by dynamic magnetic fluc-tuations only [28]. The temperature dependence of the

_{L}*in-ternal magnetic field Bi*

*μ* for EuFe2(As1*−x*P*x*)2is shown in
Fig.4*. Bi*

*μ* is proportional to the magnitude of the ordered
moment and thus to the magnetic order parameter. The
*sec-ond component (i= 2) in the μSR signal was observed only*
*for x= 1, and hence, we will discuss the x-dependence of*

the relevant physical parameters related to the first
*compo-nent (i= 1) only. For x = 0 a sharp step like increase of Bμ*1
is observed below195 K, which reflects the appearance of
*the SDW ordering of the Fe moments. The value of T*SDWis
*in good agreement with T*SDW 190 K obtained from
neu-tron diffraction [11*]. A sharp increase of B _{μ}*1 is an
indica-tion for a first order transiindica-tion. A first order transiindica-tion due
to SDW formation was also observed in the related
com-pound SrFe2As2 [29

*]. Upon lowering the temperature B*1 first tends to saturate, but increases again when the mag-netic order of the Eu2+

_{μ}*moments occurs at T*Eu. To describe

*the temperature dependence of Bμi*, we assumed the follow-ing phenomenological function:

*B _{μ}i(T )*=

*B*

_{μ,Eu}i*(0)*1−

*T*

*TEu*

*γ*1

*δ*1 +

*B*

_{μ,SDW}i*(0)*1−

*T*

*T*SDW

*γ*2

*δ*2

*,*(3)

*where B _{μ,Eu}i*

*(0) and B*

_{μ,SDW}i*(0) represent the*zero-temper-ature values of the internal magnetic field probed by the muons in the Eu and in the SDW ordered states, respectively.

*γ*

*and δ are empirical exponents. As indicated by the solid*lines in Fig.4the function in Eq. (3) describes the data rea-sonably well, yielding the parameters given in Table1. Note

*that with increasing x the values of T*SDW

*and B*1

_{μ,SDW}*(0)*

*de-crease, and for x= 0.2 and x = 1 no long-range SDW order*

*of the Fe moments is observed. On the other hand, T*Eu

*de-creases with increasing x, reaches minimum at x= 0.12 and*then increases again, in agreement with the above

*suscepti-bility measurements. In addition, B*1

_{μ,Eu}*(0) significantly*

*in-creases with x above x= 0.12. Considering the*

*magnetiza-tion results, the increase of B*1

_{μ,Eu}*(0) may be ascribed to the*appearance/growth of the ferromagnetic component as a re-sult of P substitution. However, without microscopic

*mod-eling (i.e., calculation of the μ stopping site and the*

*dipo-lar fields at the μ site) it is not possible to conclude how a*change of the magnetic structure with P substitution would affect the internal field at the muon site.

The temperature dependences of the transverse and
*lon-gitudinal depolarization rates λ*1_{T}*and λ*1* _{L}* are presented in
Fig.5

*(a) and (b), respectively. Note that λ*1

*is much smaller*

_{T}*for the end members x*= 0, 1 of the investigated system

*than for the mixed compounds x= 0.12, 0.2. As shown*in Fig. 5

*(a), for x*= 0, 0.12, and 0.2, the onset of the

*Fe magnetic order is accompanied by an increase of λ*1

*that decreases with decreasing temperature. Upon reaching*

_{T}*the magnetic ordering temperature of Eu λ*1

*shows another*

_{T}*maximum. For x= 1, the strong increase of λ*1

_{T}*around T*Eu is only due the Eu order. No SDW transition is observed at higher temperatures. The magnetic ordering temperatures of

*Eu (T*Eu

*) and Fe (T*SDW) are also clearly visible in the

*longi-tudinal relaxation rate λ*1

*, which also shows a clear anomaly*

_{L}**Table 1 Summary of the parameters obtained for the polycrystalline**

samples of EuFe2(As1*−x*P*x*)2*(x*= 0, 0.12, 0.2, 1) by means of

*mag-netization and μSR experiments. T*_{Eu}*χ* *and T*_{Eu}*μSR* are the magnetic
ordering temperatures of the Eu moments determined by susceptibility
*and μSR measurements. T*SDWdenotes the SDW ordering temperature

*of the Fe moments determined from μSR experiments. Bi*

*μ,Eu(0) and*

*Bi*

*μ,SDW(0) (i*= 1, 2) represent the zero-temperature values of the

in-ternal magnetic fields at the muon site probed in the Eu and the SDW
ordered state
*x* *T*_{Eu}*χ* (K) *T*_{Eu}*μSR*(K) *T*SDW(K) *Bμ,Eu*1 *(0) (T)* *Bμ,Eu*2 *(0) (T)* *Bμ,SDW*1 *(0) (T)* *Bμ,SDW*2 *(0) (T)*
0 19.5(6) 20.5(5) 195(3) 0.45(1) – 0.35(1) –
0.12 16.5(5) 16.7(6) 140(5) 0.476(12) – 0.258(10) –
0.2 17.9(5) 18.4(2) 85 0.997(12) – 0 –
1 29.5(5) 29.3(4) 0 1.08(1) 1.37(2) 0 0

* Fig. 5 (a) Transverse relaxation rate λ*1

*(T) for the samples EuFe2(As1*

_{T}*−x*P

*x*)2

*with x*= 0, 0.12, 0.2, and 1. Lines are guides to

* the eye. (b) Longitudinal relaxation rate λ*1

*(T) for EuFe2(As1*

_{L}*−x*P

*x*)2

*(x= 0, 0.12, 0.2, 1). The arrows mark the transition temperatures for*
*the high-temperature SDW (T*SDW) and the low-temperature Eu order

*(T*Eu)

*at T*Eu*and T*SDW(see Fig.5(b)). As mentioned above, for the
*sample with x= 0.2 (see Fig.*3(c), diamonds) only a fast
*de-polarization of the implanted muons is observed above T*Eu,
but no coherent precession signal. The fast depolarization of
*the μSR signal could be either due to a wide distribution*
of static fields, and/or to strongly fluctuating magnetic
mo-ments. To discriminate between these two possibilities we
*compare the values of λ*1_{T}*and λ*1_{L}. Note that for x= 0.2,*and T < 85 K λ*1* _{T}* is very large (50 MHz) while λ1

*is small (0.05 MHz). λ1*

_{L}*T* consists of a static as well as of
*a dynamic contribution, while λ*1* _{L}*contains only a dynamic

*contribution. Since in our case λ*1

_{T}*λ*1

*, the static*

_{L}*contribu-tion dominates λ*1

_{T}, and the fast depolarization of the μSR*signal observed for x= 0.2 is due to the (quasi-)static*

*dis-ordered SDW phase with T*SDW 85 K. The important pa-rameters for all samples extracted from the magnetization

*and the μSR experiments are summarized in Table*1.

*Very recently, bulk superconductivity with T*c 28 K
was reported in single crystals of P substituted
EuFe2(As1*−x*P*x*)2 [19] based on resistivity, magnetization,
and specific heat measurements. However,
superconductiv-ity coexisting with AFM Eu2+ order was only found in a
*very narrow x range (0.16≤ x ≤ 0.22), where the SDW*
transition is suppressed. In the present study, no indication
*of superconductivity was seen for x= 0.2 from *
magneti-zation measurements. This might be due to the fact that in
*our sample (x= 0.2) the SDW state is not completely *
*sup-pressed as supported by the μSR measurements. In addition*
to chemical pressure, the physical properties of EuFe2As2
can be also tuned by the application of hydrostatic pressure
[6,20]. Previous reports of high pressure experiments on
EuFe2As2revealed pressure-induced superconductivity in a
narrow pressure range of 2.5–3.0 GPa [6,20], accompanied
by a suppression of the SDW state of the Fe moments. Since
pressure experiments on EuFe2As2 were already reported
by various groups [6,20], we decided to study pressure
ef-fects in the P substituted sample EuFe2(As*0.88*P*0.12*)2. The
*sample with x* *= 0.12 was chosen for the following *
rea-sons: (i) According to the SC phase diagram reported [19]
for EuFe2As2 as a function of chemical pressure (P

*con-tent x), the sample with x= 0.12 is close to the value of*
*x* at which superconductivity appears. By applying
hydro-static pressure, the SC phase might be reachable. (ii) Based
on previous reports [6,20], superconductivity was found in
the vicinity of the pressure value where the SDW state is
suppressed.

In the following sections, the results of the magnetization
*and the μSR experiments performed on EuFe*2(As*0.88*P*0.12*)2
under hydrostatic pressures are presented.

3.2 Hydrostatic Pressure Effect on EuFe2(As*0.88*P*0.12*)2
*3.2.1 High Pressure Magnetization Measurements*

Magnetization measurements were carried out under
*hydro-static pressures up to p* *= 5.9 GPa. The temperature *
*de-pendence of the ZFC and FC magnetic susceptibilities χ*
for EuFe2(As*0.88*P*0.12*)2 recorded at ambient and selected
applied pressures is shown in Fig. 6*(a) (p≤ 0.4 GPa), in*
Fig. 6(b) (0.42 GPa*≤ p ≤ 0.55 GPa), and in Fig.* 6(c)
(1.1 GPa*≤ p ≤ 5.9 GPa). Note that Fig.*6shows the data
after subtraction of the background signal from the empty
*pressure cell. The magnetic ordering temperature T*Euof the
Eu2+moments was determined as described in Sect.3.1.2.
At ambient pressure, a clear bifurcation between the ZFC
*and FC curves appears below T*Eu* 16.5 K, which is *
con-sistent with the susceptibility data obtained for the sample
without pressure cell (see Fig. 2). In addition, the
mag-nitudes of the susceptibilities are also in fair agreement.
Upon increasing the pressure, an anomaly in the ZFC
*sus-ceptibility is observed at p= 0.4, 0.42, and 0.48 GPa as*
shown in Fig. 6(a) and (b). The low-temperature data for
*p* *= 0.4 GPa are shown in the inset of Fig.* 6(a). In
ad-dition to the Eu order observed at 18 K, a strong
de-crease of the ZFC susceptibility is observed at 11 K,
which is possibly due to the appearance of
superconductiv-ity. The decrease of the susceptibility corresponds to nearly
100 % diamagnetic shielding. In order to confirm
supercon-ductivity, transport measurements under pressure are
nec-essary. Just magnetization data do not allow to conclude
*that the observed decrease of χ*ZFC is due to the
appear-ance of superconductivity. Hence we call this phase “X”.
*For p* *= 0.42 GPa, the susceptibility also shows a *
*pro-nounced decrease at T*X 20 K (see Fig. 2(b), the
low-temperature data are shown in the inset). Below 18.2 K,
the susceptibility starts to increase again due to the C-AFM
ordering of the Eu2+ moments. Upon increasing the
*pres-sure to p= 0.47 GPa, the transition temperature T*X
*de-creases to 8.8 K. Above p* *= 0.55 GPa, the “X” phase*
is no longer visible (see Fig. 6(c)). It is also absent for
*p <0.35 GPa. Therefore, pressure-induced “X” phase in*
EuFe2(As*0.88*P*0.12*)2 is very likely present in a very
*nar-row pressure range. We observed that T*Eu increases upon

**Fig. 6 Temperature dependence of the ZFC and FC magnetic **

suscep-tibility of EuFe2(As*0.88*P*0.12*)2 *in a magnetic field of μ*0*H*= 2 mT

*for p ≤ 0.4 GPa (a), for 0.42 GPa ≤ p ≤ 0.55 GPa (b), and for*
1.1 GPa

**≤ p ≤ 5.9 GPa (c). The arrows mark the ordering***tempera-ture of Eu moments (T*Eu

*) and the “X” transition temperatures (T*X).

**The insets of panels (a) and (b) show the low temperature data for**

*p= 0.4 GPa and 0.42 GPa, respectively, illustrating the transition to*

*the superconducting state marked by the arrows. The solid lines are*
guides to the eye

increasing hydrostatic pressure, similar to chemical
*pres-sure. The maximum value of T*Eu = 56 K is reached at
*p= 5.6 GPa, and at higher pressures it tends to decrease*
(see Fig.6*(c)). For instance, T*Eu= 53 K at the maximum
*applied pressure p= 5.9 GPa. A maximum of T*Euwas also

**Fig. 7 ZF μSR spectra of**

EuFe2(As*0.88*P*0.12*)2measured

*at p= 0.0, 0.66, 1.1, and 2 GPa,*
recorded for three different
*temperatures: T < T*Eu*(circles),*

*T*Eu*< T < T*SDW*(diamonds),*

*and T > T*SDW*(spheres). The*

*solid lines represent fits to the*

data by means of Eq. (4)

observed for the parent compound EuFe2As2, but at higher
*pressure (p*= 8 GPa). According to recent X-ray
diffrac-tion studies [30] of EuFe2As2, a collapsed tetragonal (cT)
phase was found above 8 GPa. It is known that the
pressure-induced structural transition toward the cT phase is
con-nected with a valence change of the Eu ions, as reported for
EuFe2P2and EuCo2P2[31]. Therefore, it is possible that the
*decrease of T*Euabove 5.6 GPa is connected with a
pressure-induced valence change from the magnetic Eu2+to the
non-magnetic Eu3+ state. However, to gain further insight into
*this pressure region, measurements at p > 5.9 GPa are *
nec-essary.

*3.2.2 Zero-Field μSR Measurements Under Pressure*
Hydrostatic pressure effects on the magnetic properties
of EuFe2(As*0.88*P*0.12*)2 were studied microscopically by
*means of ZF μSR. Some representative μSR time spectra at*
different applied pressures are shown in Fig.7. A
*substan-tial fraction of the μSR asymmetry signal originates from*
muons stopping in the MP35N pressure cell [23]
*surround-ing the sample. Therefore, the total μSR asymmetry is a*
sum of two components:

*A*ZF*(t )= A*ZF_{S} *(t )+ A*ZF_{PC}*(t ),* (4)
*A*ZF_{S} *(t )is the contribution of the sample, and A*ZF_{PC}*(t )*is the
*contribution of the pressure cell. A*ZF_{S} *(t )* is well described

by Eq. (2*) with α*1*= 2/3 and β*1*= 1/3 (since for x = 0.12*
*the μSR spectra contain only one frequency, α*2= 0 and
*β*2= 0). The signal of the pressure cell was analyzed by a
damped Kubo–Toyabe (KT) function [23]:

*A*ZF_{PC}*(t )= A*ZF_{PC}*(0)*
1
3+
2
3*(*1*− σ t)e*
*−σ*2* _{t}*2

_{/2}*e−λt.*(5)

*Here A*ZF_{PC}*(0) is the amplitude of A*ZF_{PC}*(t )at t*= 0. The width
*of the static Gaussian field distribution σ* *= 0.338 µ s*−1
*and the damping rate λ= 0.04 µ s*−1 were obtained from
a measurement of the empty pressure cell. The total
*ini-tial asymmetry is A*ZF_{S} *(0)* *+ A*ZF_{PC}*(0)* *= 0.29. The ratio*
*A*ZF_{S} *(0)/[A*ZF_{S} *(0)+ A*ZF_{PC}*(0)] 40 % implies that *
approxi-mately 40 % of the muons are stopping in the sample. Up
*to p= 1.1 GPa the spontaneous muon-spin precession in*
the Eu ordered and in the SDW state is clearly observed
*in the ZF μSR time spectra (see Fig.* 7), indicating long
range magnetic order in the Eu and the Fe sublattice. Above
*p= 1.1 GPa the SDW state is suppressed and only the*
magnetic order of the Eu moments remains. The
*tempera-ture dependence of the internal field B _{μ}*1 for various
hydro-static pressures is shown in Fig.8

*. The inset shows B*1 at low temperatures where the magnetic ordering of the Eu2+ moments is evident. The data were analyzed by Eq. (3).

_{μ,Eu}*The SDW ordering temperature T*SDW of the Fe moments

*(T*SDW

*= 140 K at ambient pressure) as well as B*1 created by the Fe sublattice decrease with increasing

_{μ,SDW}*pres-sure. Above p= 1.1 GPa, the SDW order is completely*

*suppressed. On the contrary, T*Eu increases with pressure,

in agreement with the susceptibility measurements. In
*addi-tion, B _{μ,Eu}*1 related to the Eu ordered state also increases with

*pressure. Note the sharp increase of B*1

_{μ,Eu}*below T*Euwith

*increasing the pressure from p= 0 GPa to p = 0.44 GPa.*

*For p > 0.44 GPa, a more smooth increase of B*1 is observed. Relevant parameters of EuFe2(As

_{μ,Eu}*0.88*P

*0.12*)2

*tracted from the high pressure magnetization and μSR*ex-periments are listed in Table2.

As shown above the magnetization measurements indi-cate the presence of a possible SC phase in the pressure

* Fig. 8 Temperature dependence of the internal field B*1

*μ*at the muon

site for the sample EuFe2(As*0.88*P*0.12*)2 recorded at various applied

*pressures. The solid lines represent fits to the data by means of Eq. (*3).

*The arrows mark the ordering temperature T*SDW*. The inset shows the*

*low temperature data, illustrating the transition at T*Euto the

magneti-cally ordered state of the Eu moments

range 0.36 GPa*≤ p ≤ 0.5 GPa. An attempt to detect it in the*
sample EuFe2(As*0.88*P*0.12*)2*with ZF and TF μSR, failed *
be-cause of the strong intrinsic magnetism present in the
sam-ple.

**4 Phase Diagram**

Figure9*(a) shows the (x–T ) phase diagram for the system*
EuFe2(As1*−x*P*x*)2. The *(p–T )* phase diagram of
EuFe2(As*0.88*P*0.12*)2is plotted in Fig.9*(b). The data for T*Eu
represented by the triangles in Fig.9(a) are taken from [25].
*In the (x–T ) phase diagram, three different phases were*
identified: a paramagnetic phase (PM), spin-density wave
order of the Fe moments (SDW), and magnetic order of
Eu2+ * _{moments (MO). Moreover, in the (p–T ) phase }*
dia-gram, pressure-induced “X” phase was found (see the inset
of Fig.9(b)). In Fig.10

*, the internal magnetic fields B*1

_{μ,Eu}*and B*1 probed by the muons in the Eu ordered and in the SDW state and the low temperature value of the

_{μ,SDW}*mag-netic susceptibility χ*ZFC(7 K) are plotted as a function of P

*content x and applied pressure p.*

By combining the above phase diagrams, one obtains
a coherent physical picture on the system EuFe2As2 upon
P substitution and on EuFe2(As*0.88*P*0.12*)2 under
hydro-static pressure. An important finding is the observation of
pressure-induced “X” phase in EuFe2(As*0.88*P*0.12*)2,
coex-isting with magnetic order of the Eu and Fe moments.
“X” phase appears in the narrow pressure region of 0.36–
0.5 GPa. The presented phase diagrams in combination with
the results obtained for the parent compound under
pres-sure [6,20] allow us to draw the following conclusion on

**Table 2 Summary of the**

parameters obtained for the
polycrystalline sample of
EuFe2(As*0.88*P*0.12*)2at different

hydrostatic pressures by means
*of magnetization and μSR*
experiments. The meaning of
the symbols is given in the text

*p*(GPa) *T*_{Eu}*χ* (K) *T*_{Eu}*μSR*(K) *T*X(K) *T*SDW*μSR*(K) *Bμ,Eu*1 *(0) (T)* *Bμ,SDW*1 *(0) (T)*
0 16.5(5) 16.4(3) – 141.2(1) 0.44(1) 0.25(1)
0.4 17.5(4) – 11.2(3) – – –
0.42 17.6(5) – 20.3(3) – – –
0.44 – 17.7(3) - 110(1) 0.99(2) 0.19(2)
0.48 17.9(4) – 7.3(3) – – –
0.66 18.9(5) 18.4(6) 0 75(2) 1.07(5) 0.17(4)
1.1 20.5(5) 19.9(7) 0 40(3) 1.27(3) 0.12(2)
1.73 24.6(3) – 0 – – –
1.97 24.4(5) 23.6(7) 0 0 1.23(2) 0
2.5 27.2(3) – 0 – – –
3.85 35.8(5) – 0 – – –
4.54 42.5(4) – 0 – – –
5.1 49.5(3) – 0 – – –
5.6 57(4) – 0 – – –
5.9 53(5) – 0 – – –

* Fig. 9 (a) (x–T ) phase diagram of EuFe*2(As1

*−x*P

*x*)2. The data points

*represented by the triangles are taken from [*25* ]. (b) (p–T ) phase *
di-agram of EuFe2(As

*0.88*P

*0.12*)2. The various phases in the phase

dia-grams and the corresponding transition temperatures are denoted as
*follows: paramagnetic (PM), spin-density wave (SDW) and T*SDW,

*magnetic ordering of Eu (MO) and T*Eu, “X” phase (the meaning of this

*phase is given in the text) and T*X**. For clarity, the inset in (b) shows the**

“X” phase present in a very narrow pressure range

the relation between chemical and hydrostatic pressure in EuFe2As2:

*1. Both chemical and hydrostatic pressure suppress T*SDW
*and B _{μ,SDW}*1

*(0). However, the SDW ground state is*

*dif-ferently affected by x and p. At all applied pressures*

*be-low p= 1.1 GPa long-range SDW order was observed,*

*while in the case of chemical pressure for x= 0.2 a*dis-ordered SDW phase exist. This may be related to the fact that by chemical pressure (P substitution) considerably more disorder is introduced.

2. Figure 9 *shows that in the case of P substitution T*Eu
*first decreases as a function of x, reaches a minimum*
*at x= 0.12, and then increases. For a fixed P content*
*of x= 0.12, the ordering temperature T*Euincreases with
*pressures up to p= 5.6 GPa. Above p = 5.6 GPa, *

* how-Fig. 10 Zero-temperature values of the internal magnetic fields B*1

*μ,Eu*

*and B _{μ,SDW}*1 and the low-temperature value of the magnetic

*suscepti-bility χ*ZFC

**as a function of the P content x (a) and applied pressure (b)***ever, T*Eu*(p)*decreases, accompanied by a possible
va-lence change of the Eu moments. In the parent compound
EuFe2As2, a valence change was found at a higher
*pres-sure p*= 8 GPa.

*3. The internal magnetic field B _{μ,Eu}*1

*(0) in the Eu ordered*

*state increases with increasing x as well as by applying*hydrostatic pressure (see Fig.10(a)–(b)).

4. The low temperature value of the magnetic susceptibility
*χ*ZFC *(7 K) first increases with increasing x and p and*
*above some critical values (x= 0.2 and p = 1.1 GPa) it*
decreases (see Fig.10(a)–(b)).

By considering the findings listed above, the qualitative
statement can be made that the properties of
EuFe2(As1*−x*P*x*)2 are similarly tuned by chemical and
hy-drostatic pressure.

**5 Conclusions**

In summary, the magnetic and superconducting properties
of the system EuFe2(As1*−x*P*x*)2*(x*= 0, 0.12, 0.2, 1) were
*studied by magnetization and μSR experiments. In addition,*
*the sample with x= 0.12 was also investigated by applying*
*hydrostatic pressure up to p 5.9 GPa. The (x–T ) phase *
di-agram of EuFe2(As1*−x*P*x*)2*and the (p–T ) phase diagram of*

EuFe2(As*0.88*P*0.12*)2were determined and discussed as well
*as compared to the (p–T ) phase diagram recently obtained*
for EuFe2As2[6,20]. The present investigations reveal that
the magnetic coupling between the Eu and the Fe
sublat-tices strongly depends on chemical and hydrostatic pressure
*and determines the (x–T ) and (p–T ) phase diagrams as *
pre-sented in this work. According to the above discussed phase
diagrams, chemical and hydrostatic pressures have
qualita-tively a similar effect on the Fe and Eu magnetic order.

There are still some open questions related to
supercon-ductivity and its interplay with the magnetic ground state of
the system EuFe2As2. One of the most interesting aspects of
this particular member of Fe-based superconductors is the
possibility to observe coexistence or competition between
superconductivity and rare-earth Eu magnetic order. In the
present work, the so-called “X” phase induced by pressure
was observed in EuFe2(As*0.88*P*0.12*)2in addition to the
mag-netic phases of the Eu and Fe sublattices. It exists in a narrow
pressure range 0.36–0.5 GPa. This phase is possibly
super-conducting. However, transport measurements as a function
of pressure are required in order to clarify this point.

**Acknowledgements** This work was supported by the Swiss
Na-tional Science Foundation, the SCOPES grant No. IZ73Z0_128242,
*and the NCCR Project MaNEP. The μSR experiments were performed*
at the Swiss Muon Source of the Paul Scherrer Institute (PSI), Villigen,
Switzerland.

**References**

1. Kamihara, Y., Watanabe, T., Hirano, M., Hosono, H.: J. Am.
**Chem. Soc. 130, 3296 (2008)**

**2. Rotter, M., Tegel, M., Johrendt, D.: Phys. Rev. Lett. 101, 107006**
(2008)

3. Chen, X.H., Wu, T., Wu, G., Liu, R.H., Chen, H., Fang, D.F.:
**Na-ture (London) 453, 761 (2008)**

4. Torikachvili, M.S., Bud’ko, S.L., Ni, N., Canfield, P.C.: Phys. Rev.
**Lett. 101, 057006 (2008)**

5. Fukazawa, H., Takeshita, N., Yamazaki, T., Kondo, K., Hirayama,
K., Kohori, Y., Miyazawa, K., Kito, H., Eisaki, H., Iyo, A.: J. Phys.
**Soc. Jpn. 77, 105004 (2008)**

6. Terashima, T., Kimata, M., Satsukawa, H., Harada, A., Hazama,
K., Uji, S., Suzuki, H.S., Matsumoto, T., Murata, K.: J. Phys. Soc.
**Jpn. 78, 083701 (2009)**

7. Ren, Z.A., Lu, W., Yang, J., Yi, W., Shen, X.L., Li, Z.C., Che,
G.C., Dong, X.L., Sun, L.L., Zhou, F., Zhao, Z.X.: Chin. Phys.
**Lett. 25, 2215 (2008)**

8. Matsuishi, S., Inoue, Y., Nomura, T., Hirano, M., Hosono, H.:
**J. Phys. Soc. Jpn. 77, 113709 (2008)**

9. Zhao, J., Huang, Q., de la Cruz, C., Li, S., Lynn, J.W., Chen, Y.,
Green, M.A., Chen, G.F., Li, G., Li, Z., Luo, J.L., Wang, N.L.,
**Dai, P.: Nat. Mater. 7, 953 (2008)**

10. Raffius, H., Mörsen, M., Mosel, B.D., Müller-Warmuth, W., Jeitschko, W., Terbüchte, L., Vomhof, T.: J. Phys. Chem. Solids

**54, 135 (1993)**

11. Xiao, Y., Su, Y., Meven, M., Mittal, R., Kumar, C.M.N., Chatterji,
T., Price, S., Persson, J., Kumar, N., Dhar, S.K., Thamizhavel, A.,
**Brueckel, T.: Phys. Rev. B 80, 174424 (2009)**

12. Jiang, S., Luo, Y.K., Ren, Z., Zhu, Z.W., Wang, C., Xu, X.F., Tao,
**Q., Cao, G.H., Xu, Z.A.: New J. Phys. 11, 025007 (2009)**
13. Guguchia, Z., Roos, J., Shengelaya, A., Katrych, S., Bukowski, Z.,

Weyeneth, S., Murányi, F., Strässle, S., Maisuradze, A., Karpinski,
**J., Keller, H.: Phys. Rev. B 83, 144516 (2011)**

14. Sefat, A.S., Jin, R., McGuire, M.A., Sales, B.C., Singh, D.J.,
**Man-drus, D.: Phys. Rev. Lett. 101, 117004 (2008)**

15. Leithe-Jasper, A., Schnelle, W., Geibel, C., Rosner, H.: Phys. Rev.
**Lett. 101, 207004 (2008)**

16. He, Y., Wu, T., Wu, G., Zheng, Q.J., Liu, Y.Z., Chen, H., Ying,
J.J., Liu, R.H., Wang, X.F., Xie, Y.L., Yan, Y.J., Dong, J.K., Li,
**S.Y., Chen, X.H.: J. Phys. Condens. Matter 22, 235701 (2010)**
17. Li, L.J., Luo, Y.K., Wang, Q.B., Chen, H., Ren, Z., Tao, Q., Li,

Y.K., Lin, X., He, M., Zhu, Z.W., Cao, G.H., Xu, Z.A.: New J.
**Phys. 11, 025008 (2008)**

**18. Ren, Z.: Phys. Rev. B 79, 094426 (2009)**

19. Jeevan, H.S., Kasinathan, D., Rosner, H., Gegenwart, P.: Phys.
**Rev. B 83, 054511 (2011)**

20. Matsubayashi, K., Munakata, K., Isobe, M., Katayama, N.,
Oh-gushi, K., Ueda, Y., Uwatoko, Y., Kawamura, N., Mizumaki, M.,
**Ishimatsu, N., Hedo, M., Umehara, I.: Phys. Rev. B 84, 024502**
(2011)

21. Guguchia, Z., Bosma, S., Weyeneth, S., Shengelaya, A.,
**Puz-niak, R., Bukowski, Z., Karpinski, J., Keller, H.: Phys. Rev. B 84,**
144506 (2011)

**22. Rodrígues-Carvajal, J.: Physica B 192, 55 (1993)**
23. Andreica, D.: Ph.D. Thesis, IPP/ETH-Zürich (2001)
**24. Suter, A., Wojek, B.M.: Phys. Procedia 30, 69–73 (2012)**
25. Cao, G., Xu, S., Ren, Z., Jiang, S., Feng, C., Xu, Z.: J. Phys.

**Con-dens. Matter 23, 464204 (2011) (5 pp.)**

26. Zapf, S., Wu, D., Bogani, L., Jeevan, H.S., Gegenwart, P., Dressel,
**M.: Phys. Rev. B 84, 140503(R) (2011)**

27. Ryan, D.H., Cadogan, J.M., Xu, S., Xu, Z., Cao, G.: Phys. Rev. B

**83, 132403 (2011)**

28. Maeter, H., Luetkens, H., Pashkevich, Yu.G., Kwadrin, A.,
Khasanov, R., Amato, A., Gusev, A.A., Lamonova, K.V.,
Chervin-skii, D.A., Klingeler, R., Hess, C., Behr, G., Büchner, B., Klauss,
**H.H.: Phys. Rev. B 80, 094524 (2009)**

29. Jesche, A., Caroca-Canales, N., Rosner, H., Borrmann, H.,
Ormeci, A., Kasinathan, D., Klauss, H.H., Luetkens, H.,
Khasanov, R., Amato, A., Hoser, A., Kaneko, K., Krellner, C.,
**Geibel, C.: Phys. Rev. B 78, 180504(R) (2008)**

30. Uhoya, W., Tsoi, G., Vohra, Y.K., McGuire, M.A., Sefat, A.S.,
**Sales, B.C., Mandrus, D., Weir, S.T.: J. Phys. Condens. Matter 22,**
292202 (2010)

31. Ni, B., Abd-Elmeguid, M.M., Micklitz, H., Sanchez, J.P., Vulliet,
**P., Johrendt, D.: Phys. Rev. B 63, 100102 (2001)**